1 | J. Name., 2020, 00, 1-3 This journal is © The Royal Society of Chemistry 20xx
Strong Plasmon-Exciton Coupling in Bimetallic Nanoring and Nanocuboid
Na Li1,‡, Zihong Han1,‡, Yuming Huan2,‡, Kun Liang2,‡, Xiaofeng Wang1, Fan Wu2,
Xiaoying Qi1, Yingxu Shang1, Li Yu2 and Baoquan Ding1,3,4,*
1CAS Key Laboratory of Nanosystem and Hierarchical Fabrication, CAS Center for Excellence in Nanoscience, National
Center for Nanoscience and Technology, 11 BeiYiTiao, ZhongGuanCun, Beijing 100190, China
2State Key Laboratory of Information Photonics and Optical Communications, Beijing University of Posts and
Telecommunications, 10 Xitucheng Road, Beijing, 100876, China
3University of Chinese Academy of Sciences, Beijing 100049, China
4School of Materials Science and Engineering, Zhengzhou University, Zhengzhou 450001, China
E-mail: [email protected]
‡These authors contributed equally to this work.
Materials and Methods
Materials. H2O2 (30 wt %) was purchased from Aladdin. Acetonitrile was purchased from Fisher
Chemical. Sodium citrate (SC), Silver nitrate (AgNO3), Sodium borohydride (NaBH4), L-ascorbic acid
(AA), Hydroxylamine hydrochloride (Hya), sodium hydroxide (NaOH), hydrogen tetrachloroaurate (III)
trihydrate (HAuCl4·3H2O), bis(p-sulfonatophenyl)-phenylphosphine dihydrate dipotassium (BSPP),
hexadecylpyridinium chloride monohydrate (CPC), 5,6-Dichloro-2-[[5,6-dichloro-1-ethyl-3-(4-
inner salt (TDBC), Cetyltrimethyl Ammonium Bromide (CTAB) were purchased from Sigma-Aldrich. All
chemicals were used as received without further purification. Ultrapure water obtained from a Milli-Q
system was used in all experiments. All glassware was cleaned using freshly prepared aqua regia (HCl:
HNO3 in a 3:1 ratio by volume) and copious amounts of deionized water.
Synthesis of Au Nanorings. Au nanorings were fabricated through a template method by selective Au
deposition on the edges of silver nanoplates and subsequent Ag etching, followed by a second Au
deposition. Details are as follows:
Preparation of Ag Nanoplates. Ag nanoplates were prepared according to previous literature with some
modification. First, Ag seeds were prepared as follows: To 200 mL of deionized water (DIW), aqueous
solutions of sodium citrate (0.0045 M), silver nitrate (1 × 10−4 M), and 480 μL H2O2 (30 wt %) were added,
Electronic Supplementary Material (ESI) for Journal of Materials Chemistry C.
This journal is © The Royal Society of Chemistry 2020
2 | J. Name., 2020, 00, 1-3 This journal is © The Royal Society of Chemistry 20xx
followed by adding an icecold, fresh prepared aqueous solution of sodium borohydride (0.1 M 1.2 mL)
with vigorous stirring. After 5 min of stirring, the solution was left undisturbed for 2 h in 4 °C. The
synthesized Ag nanoseeds were concentrated by centrifugation before use. Second, Ag nanoplates were
prepared as follows: To 44 mL of deionized water (DIW), 20 mL of acetonitrile, 300 μL of ascorbic acid
(0.1 M), 200 μL sodium citrate (0.075 M), and Ag seeds were added, followed by adding 240 μL of silver
nitrate (0.1 M) with vigorous stirring for 30 min. The Ag nanoplates were centrifuged and washed with
water for future use.
Preparation of Au Nanorings. Au nanorings were prepared according to previous literature with some
modifications. First, [email protected] nanoplates were prepared as follows: Basic hydroxylamine hydrochloride
solution (3 mM) was prepared. The as-prepared Ag nanoplates were dissolved in 20 mL of water in a glass
container placed in an ice bath. To this solution, the basic hydroxylamine hydrochloride and an aqueous
solution of hydrogen tetrachloroaurate (III) trihydrate (HAuCl4·3H2O, 0.3 mM) were added via syringe
pump at a rate of 2 mL/h with vigorous stirring. After 30 mins, The [email protected] nanoplates were centrifuged.
Secondly, the thin Au nanorings were prepared as follows: The as-prepared [email protected] nanoplates were
incubated with 5 mL solution of bis (p-sulfonatophenyl)-phenylphosphine dihydrate dipotassium (BSPP, 2
mM) to etch the Ag templates. The reaction was monitored by UV-vis spectroscopy to indicate the
completion of etching. The resulting thin Au nanorings were centrifuged. Finally, to prepare thicker Au
nanorings, the thin Au nanorings were dispersed in 20 mL of water. The above basic hydroxylamine
hydrochloride solution and aqueous solution of HAuCl4·3H2O were added via syringe pump at a rate of 2
mL/h with vigorous stirring. The reaction was monitored by UV-vis spectroscopy to determine the
thickness of Au nanorings.
Synthesis of [email protected] core-shell nanorings structure. In a typical method, 100 μL of the Au nanorings
(0.5 nM) and 16 μL of CPC aqueous solution (0.1 M) were mixed together. Then, different amounts (2-15
μL) of AgNO3 (10 mM) and 8 μL of AA (0.1 M) were added consecutively. The mixture was heated up to
60 °C for 1 h then cooled to room temperature. The as-synthesized [email protected] nanorings were centrifuged at
5000 rpm for 3 min and resuspended in deionized water (DIW).
Preparation of [email protected] nanorings/J-aggregate hybrids. We prepared monodisperse [email protected]
nanorings/J-aggregate hybrids based on the previous work with some modifications.1-5 We directly coated
CPC-stabilized [email protected] nanorings with TDBC without supplementary addition of salts or bases during the
3 | J. Name., 2020, 00, 1-3 This journal is © The Royal Society of Chemistry 20xx
synthesis and carried out at room temperature. The fabrication of [email protected] nanorings/J-aggregate hybrids
based on electrostatic self-assembly. This simple preparation process is also reproducible allowing
sufficient, high quality [email protected] nanorings/J-aggregate hybrids to be made for photonic applications. The
experimental details are attached below: The as-prepared [email protected] nanorings were incubated with 5 μL of
TDBC (5 mM) for 1 h. Then the resulting samples were centrifuged and washed twice with water.
Synthesis of Au Nanorods. The gold nanorods were synthesized via a seed-mediated growth method. The
seed solution for Au nanorods was prepared as reported previously. A 5 mL amount of 0.5 mM HAuCl4
was mixed with 5 mL of 0.2 M CTAB solution. A 0.6 mL portion of fresh 0.01 M NaBH4 was diluted to 1
mL with water and was then injected into the Au (III)-CTAB solution under vigorous stirring (1200 rpm).
The solution color changed from yellow to brownish-yellow, and the stirring was stopped after 2 min. The
seed solution was aged at room temperature for 2 h before use. To prepare the growth solution, 0.9 g of
CTAB together with 0.08 g of sodium salicylate were dissolved in 25 mL of warm water (70°C) in a 500
mL Erlenmeyer flask. The solution was allowed to cool to 30°C, then a 600 μL of 4 mM AgNO3 solution
was added. The mixture was kept undisturbed at 30 °C for 15 min, after which 25 mL of 1 mM HAuCl4
solution was added. After 15 min of slow stirring (400 rpm), 1mL of 0.064 M ascorbic acid was added, and
the solution was vigorously stirred for 30 s until it became colorless. Finally, 80 μL of seed solution was
injected into the growth solution. The resultant mixture was stirred for 30 s and left undisturbed at 30 °C
for 12 h for Au nanorods growth. The reaction products were isolated by centrifugation at 3000 rpm for 15
min followed by removal of the sediment to remove Au nanoparticles. And then the reaction products were
isolated by centrifugation at 8500 rpm for 15 min followed by removal of the supernatant, and washed once
Synthesis of [email protected] core-shell nanocuboids structure. In a typical method, 100 μL of the Au nanorods
(0.5 nM) and 16 μL of 0.1 M CPC aqueous solution were mixed together. Then, different amounts (0.5-5
μL) of 10 mM AgNO3 and 8 μL of 0.1 M AA were added consecutively. The mixture was heated up to 60
°C for 1 h then cooled to room temperature. The as-synthesized [email protected] nanocuboids were centrifuged at
8600 rpm for 3 min and re-suspended in deionized water (DIW).
Preparation of [email protected] nanocuboids/J-aggregate complex. The as-prepared [email protected] nanocuboids were
incubated with 5 μL of TDBC (5 mM) for 1 h. Then the resulting samples were centrifuged and washed
twice with water.
4 | J. Name., 2020, 00, 1-3 This journal is © The Royal Society of Chemistry 20xx
Optical characterization. Extinction spectra were measured using a Shimadzu UV-2450 UV-vis
spectrophotometer. The scanning was carried out at a range of 230-900 nm at room temperature in a 1 cm-
length cell and the scan rate was 300 nm/min.
TEM characterization. Before depositing the sample solution, the grids were first glow discharged using
Emitech K100X machine in order to increase its hydrophilicity. The samples for TEM imaging were
prepared by placing 5 μL of the sample solution on a carbon-coated copper grid (300 meshes, Ted Pella).
After 10 min of deposition, the unbound sample was wicked away from the grid using filter paper. To
remove the excess salt, the grid was touched with a drop of water, and the excess water was wicked away
using filter paper. The